ISSN Print: 2327-4077
DOI: 10.4236/jmmce.2018.63027 May 21, 2018 382 J. Minerals and Materials Characterization and Engineering
Removal of Silica and Alumina as Impurities
from Low-Grade Iron Ore Using Wet
High-Intensity Magnetic Separation
and Reverse Flotation
, Moses Charles Siame, Atsushi Shibayama
Graduate School of International Resource Science, Akita University, Akita, Japan
This study investigates the removal of silica and alumina as impurities from hematite based low-grade iron ore containing 34.18 mass% iron, 31.10 mass% of silica and 7.65 mass% alumina. Wet high-intensity magnetic separation (WHIMS) and reverse flotation (RF) were investigated. In WHIMS process, 93.08% of iron was recovered with a grade of 53.22 mass% at an optimum magnetic density of 10,000 mT, and pulp density of 2% used the L-4 machine. In RF experiments, optimal results showed 95.95% of iron recovered with 51.64 mass% grade using 1 kg/t of 1% alkaline starch as iron depressant and 1:1 mixture ratio of 0.75 kg/t DAA and NaOL as silica and alumina collectors. The designed multi-stage process involving feeding the concentrate from WHIMS into RF process reduced silica to 2.02 mass%, alumina to 1.04 mass% whilst recovering 81.94% of the iron with 67.27 mass% grade. As a result of this research, a process to produce high quality iron concentrate from hema-tite based low-grade iron ore with high iron recovery rate was constructed.
Iron Ore, Hematite, Magnetic Separation, Reverse Floatation, Multi-Stage Process
The increase in demand for iron in the steelmaking industries and the depleting high-grade iron ores has led to the alternative extraction of iron from hematite based low-grade ores . The low-grade iron ores contain higher grades of silica How to cite this paper: Haga, K., Siame,
M.C. and Shibayama, A. (2018) Removal of Silica and Alumina as Impurities from Low-Grade Iron Ore Using Wet High- Intensity Magnetic Separation and Reverse Flotation. Journal of Minerals and Mate-rials Characterization and Engineering, 6, 382-394.
Received: April 23, 2018 Accepted: May 18, 2018 Published: May 21, 2018
Copyright © 2018 by authors and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0).
DOI: 10.4236/jmmce.2018.63027 383 J. Minerals and Materials Characterization and Engineering and alumina as gangue mineral assemblages with oxides of phosphorus existing in small quantities . In this study, Sanje ore of Nampundwe area of Zambia containing 31.10 mass% grade of iron and more than 38 mass% silica-alumina gangue minerals as impurities was used. The ore contains high alumina and sili-ca and it is to be used as feed in steelmaking; however these impurities adversely affect the production of pig iron and steel . High silica and alumina also form high viscous slag with greater volume in blast furnaces which requires more flux . Therefore, these impurities need to be removed before feed into the steel making process.
Magnetic separation and flotation are the two commonly used iron beneficia-tion processes and selecting the most effective process to treat low-grade ore de-pends mainly on the mineralogical structure of the ore especially the aggregation of Iron with gangue minerals . Magnetic separation using wet high-intensity technique has become one of the most suitable methods for recovery of iron from low-grade ores , due to its better separation efficiency as compared to dry magnetic separation and gravity separation . Flotation processes using either cationic or anionic collectors are therefore considered as the more most effective methods to separate iron-gauge minerals which are aggregated together and are weak magnetic particles . Many studies on reverse magnetic flotation put across performances comparison between anionic and cationic collectors in terms of iron recovery and gangue separation efficiencies. In many cases, anionic collectors have lower recovery efficiencies due to poor selectivity while cationic exhibits low efficiency due to high viscosity and low foam mobility . Cationic reverse flotation is usually pH dependent process and is done effectively at lower pH range from pH 9 to 10 as compared to anionic flotation which is done for pH range from pH 11 to pH 12 (Ana et al., 2017) . However, even with these technologies, it could not build a capable process of collecting high grade iron concentrate with high iron recovery from hematite-based ores.
This research aimed at designing a process to produce iron concentrate with minimal silica-alumina content of less than 7 mass% and higher iron grade of more than 60 mass% to meet both market requirement and production target. Wet high-intensity magnetic separation (WHIMS) was investigated; however it could not completely remove the silica-alumina gangue particles entrapped and aggregated with iron particles. Reverse flotation using cationic, anionic collec-tors and their combination also were investigated. The multi-stage separation processes were designed and compared and the best process with less metal loss for impurity removal was established based on experimental results.
2.1. Sample Preparation
flu-DOI: 10.4236/jmmce.2018.63027 384 J. Minerals and Materials Characterization and Engineering orescence spectrometer (XRF, ZSX Primus II Rigaku). Table 1 shows that the ore also contains silica and alumina of 31.10 mass% and 7.65 mass% respective-ly. Mineralogical analysis was done using RINT Rigaku X-ray diffractometer as results shown in Figure 1. The ore contains hematite (Fe2O3), silica (SiO2) and small amount of magnetite (Fe3O4).
2.2. Procedure for Magnetic Separation
All magnetic separation experiments were done using the Series L Model 4 (L-4 Machine) laboratory magnetic Separator (Eriez Magnetics Co. Ltd.). Wire mesh (expand metal) or pipe matrix fixed inside the casing of L-4 machine were used as magnetic particle collectors. The effect of magnetic flux density on silica and alumina removal was first investigated by adjusting for 3000, 5000, 7500 and 10,000 mT while pulp density and pulp flow were kept constant at 2% and 7 L/min respectively. The value of the magnetic flux density indicates the value obtained by measuring the magnetic flux density at the center of the collection box filled with the matrix. The effect of feed pulp density on iron recovery inves-tigated by adjusting the density of slurry fed into the machine to 2%, 2.5%, 5%, 7.5% and 10% at the optimum magnetic field intensity obtained from the first stage while keeping the pulp flow of 7 L/min.
Table 1. Chemical composition of Sanje Iron ore (analysed by XRF).
%Fe2O3 (Fe) %Al2O3 %SiO2 %P %MgO
48.90 (34.18) 7.65 31.10 0.05 1.33
DOI: 10.4236/jmmce.2018.63027 385 J. Minerals and Materials Characterization and Engineering
2.3. Procedure for Reverse Flotation
Flotation experiments were carried out using 237 FL flotation machine (Mekhar-Tekhnika Corp.) with 500 mL capacity, mixing at 900 rpm and 0.5 L/min of air injected. The effect of pH, collector dosage, iron depressant (starch) dosage were studied to establish best flotation parameters. 0.1% of sodium oleate (NaOL) was used as an anionic collector and 0.1% dodecyl amine acetate (DAA) as a cationic collector. Alkaline starch prepared by 1% starch (C18H32O16) and 0.1% sodium hydroxide solution mixed to 1:1 molar ratio was used as an iron depressant and methyl isobutyl carbinol (MIBC) was used as frother.
3. Results and Discussion
3.1. Magnetic Separation3.1.1. Effect of Magnetic Density
The effect of magnetic density on iron recovery and gangue removal was inves-tigated at constant pulp flow using the expand metal as magnetic collector in Figure 2. Recovery of iron and its grade increased with increase in magnetic in-tensity. Evidently, iron recovery improved from 76% to 93% with an increase in magnetic field density from 3000 mT to 10,000 mT. Silica content in the con-centrate was reduced to 18.79 mass% at 10,000 mT as compared to 19.98 mass% at 3000 mT. Increase in the magnetic field beyond 10,000 mT resulted in de-creased recovery due to the buildup of magnetic particles on matrix  .
3.1.2. Effect of Feed Pulp Density
Figure 3 shows that recovery of iron decreased from 93% to 91% for pulp den-sity of 2% to 2.5% at constant magnetic field denden-sity of 10,000 mT. Further in-crease in pulp density caused a relatively decreasing trend in iron recovery and lower silica-alumina gangue removal. The optimum pulp density was obtained at
Figure 2. Changing of iron recovery and grade as a function of magnetic density on
DOI: 10.4236/jmmce.2018.63027 386 J. Minerals and Materials Characterization and Engineering 2.5% at which 89% of iron was recovered with the grade of 49.72 mass% having 4.19 mass% alumina and 18.08 mass% of silica. At 2.5% the solid-liquid ratio at which the magnetic forces dominated over the liquid drag force. Lower pulp density increased pulp flow reduced the probability at which the particles were induced and captured by the matrix. Alternatively, higher pulp flow caused overcrowding on the matrix and reduced separation efficiency  .
3.1.3. Effect of Matrix
Figure 4 shows effect of matrix equipment on recovery and grade. The optimum magnetic field density of 10,000 mT and feed pulp 2.5% was used to investigate
Figure 3. Changing of iron recovery and grade as a function of pulp density on WHIMS
(conditions: magnetic density 10,000 mT, pulp flow rate 7 L/min, matrix expand metal).
Figure 4. Changing of iron recovery and grade as a function of pulp density on WHIMS
DOI: 10.4236/jmmce.2018.63027 387 J. Minerals and Materials Characterization and Engineering the effect of matrix equipment. Iron with grade of 49.70 mass% and recovery of 89% was obtained for the expand metal while 93% was recovered using the pipe matrix. The iron grade also showed the higher content of 51.38 mass% when the pipe matrix was used as compared to the expand metal. This result shows that the pipe matrix has a simple structure compared with the expanded metal, hence the entrainment of silica and alumina was low and the iron minerals could be ef-ficiently recovered.
3.2. Reverse Flotation3.2.1. Effect of Slurry pH
Figure 5 shows the effect of pH on the flotation of silica and alumina using DAA as cationic collector. Silica trend shows its lowest content of 31 mass% in con-centrate at pH 8 and it was not removed with further increase in pH. Iron grade trend shows a slight increase from pH 6.8 to 8. Further increase of pH from 8 to pH 10 shows a relatively constant trend on Iron grade. The reaction mechanism of alumina and silica with amine collectors depends on the surface charge of the mineral particles . The overall mineral surface charge in slurry strongly de-pends on the pH of the slurry . When surface charge and the zeta potential of the hematite are more negative, the hydrophobicity of quartz increases. In-crease in hydrophobicity of quartz during hematite flotation is attributed to more silicates attracted to cationic collectors and consequently increased sili-ca-alumina recovery in the froth . Recovery of Iron shows a constant trend also with an increase in pH, this indicates that there was no direct dependence on pH for the flotation of silica and alumina using DAA collector alone.
3.2.2. Effect of DAA Dosage
The effect of DAA collector dosage on flotation of silica and alumina was
Figure 5. Changing of iron recovery and grade as a function of pH on reverse flotation
DOI: 10.4236/jmmce.2018.63027 388 J. Minerals and Materials Characterization and Engineering investigated. The results in Figure 6 show that there was no iron recovered when 0.25 kg/t of DAA collector was consumed. Increase in collector dosage from 0.50 kg/t to 1 kg/t using 0.1% DAA shows increase in iron recovery with over 76% iron recovered for 1 kg/t DAA consumption. More alumina and silica was also removed as collector dosage was increased from 0.50 to 0.75 kg/t. Further addi-tion of 0.1% DAA showed no further alumina reducaddi-tion which implies that 0.75 kg/t of 0.1% DAA was sufficient to allow the formation of a monolayer coat on alumina particles hence allowing it together with small silica bearing particles to report to the froth .
More floatation experiments were done using sodium oleate (0.1% NaOL) collector in addition to DAA collector to improve the adsorption selectivity and consequently increase the ejection efficiency of silica and alumina .
Iron recovery shows an increasing trend with the addition of the NaOL as shown in Figure 7. The Iron recovery increased from 68.45% when DAA has used alone to 76.24% when the collector mixture of DAA and NaOL of 1:1 ratio was used. The suitable molar ratio was obtained at 1:2 which corresponds to the lowest silica content of 28 mass%. Further addition of NaOL showed a relatively decreasing trend for both Iron grade and silica floatability.
3.2.3. Effect of Starch Depressant
To remove iron from floating together with silica and alumina, dextrin starch was used as a depressant. Additionally, 0.2 kg/t of CaO was added as activator of SiO2. Figure 8 shows that iron grade increased with increase in starch dosage from 46.90 to 51.64 mass%. More alumina was reduced at 1 kg/t consumption with 2.90 mass% remaining in the concentrate. Silica showed an improved re-duction with increase in starch dosage with 20.60 mass% content in the concen-trate and considerably optimum starch dosage of 1 kg/t. On the other hands,
Figure 6. Changing of iron recovery and grade as a function of DAA dosage on reverse
DOI: 10.4236/jmmce.2018.63027 389 J. Minerals and Materials Characterization and Engineering
Figure 7. Effect of collector mixture on reverse flotation (conditions: DAA 0.75 kg/t, pH
8, MIBC 0.05 kg/t).
Figure 8. Effect of starch on flotation behavior of iron mineral, silica and almina
(condi-tions: DAA 0.75 kg/t, NaOL 0.75 kg/t, CaO 0.2 kg/t, MIBC 0.05 kg/t).
iron recovery decreased from 98.46% to 95.95% with increased dosing from 0.25 to 1 kg/t. Similarly, Silica and alumina also were reduced with an increase in al-kaline starch dosage to 20.60% and 2.90% respectively.
DOI: 10.4236/jmmce.2018.63027 390 J. Minerals and Materials Characterization and Engineering
Figure 9. FT-IR spectra of feed sample and tailing obtained from flotation.
rocking vibration at 779 cm−1, a bending asymmetric peak of C-H bond at 1344 cm−1 and a small stretch at 1574 cm−1 characterizing the CH3 bond .
Adsorption of starch on hematite alters the surface charge of iron oxide to hydrophilic condition. Hydrophobicity of iron surface allows the iron oxide to settle as underflow and remain unattached to water bubbles floating silica and alumina. The adsorption of starch on iron particles was enhanced by the use of dodecyl amine acetate (DAA) as cationic surfactant for quartz-alumina particles. DAA was also used as a cationic collector whose interaction with silica-alumina particles resulted in the formation of a repulsive charge on iron bearing particles.
3.3. Comparison of Combination Process of Magnetic
Separation and Reverse Flotation
DOI: 10.4236/jmmce.2018.63027 391 J. Minerals and Materials Characterization and Engineering mass% of alumina and 15.80 mass% of silica containing in the concentrate. The flowchart of combination process of magnetic separation of reverse flotation shows in Figure 10. The magnetic separation followed by flotation process which recovered 89.50% of iron having a higher grade of 67.27 mass%. Silica and alumina were reduced to 2.04 and 1.04 mass% respectively. More alumina and silica were removed during magnetic separation followed by flotation process because the iron-silica and iron-alumina aggregated minerals were separated more by their difference in floatability  because there are weak magnetic particles and was difficult to separate them during two stage magnetic separa-tion.
The mineral processing technique for effective removal of impurities from Sanje
Table 2. Composition of concentrates and iron recovery by two stage separation
Combination process Iron concentrate, mass% %
Fe Al2O3 SiO3 Fe recovery
Magnetic separation-Magnetic separation 67.07 1.30 2.14 92.87
Reverse flotation-Reverse flotation 55.53 2.60 15.80 87.65
Magnetic separation-Reverse flotation 67.27 1.04 2.02 89.50
Figure 10. The proposed combination process of magnetic separation and reverse
DOI: 10.4236/jmmce.2018.63027 392 J. Minerals and Materials Characterization and Engineering Iron ore was established and therefore this study concludes that;
1) Effective removal of impurities from Sanje ore using wet high-intensity magnetic separation requires lower feed pulp density of 2.5% and higher mag-netic field intensity of 10,000 mT. However, higher Iron grade with minimum impurities is not attained by single magnetic separation process with just up to 53.22 mass% iron grade attained with 12.01 mass% silica and 3.94 mass% of alumina.
2) Reverse flotation using a mixture of cationic and anionic collectors (dodecyl amine acetate (DAA) and sodium oleate (NaOL)) shows a better silica-alumina gauge removal than when only DAA is used. However, it requires the use of starch as iron depressant.
3) A combined process of magnetic separation and reverse flotation is effec-tive for removal of silica and alumina from Sanje ore. As proposed circuit, iron grade of obtained concentrate was 67.27 mass% and 81.94% of iron was recov-ered. Much of silica is reduced to 2.02% and alumina 1.04% remaining in the concentrate.
As a result of this research, a process to produce high quality iron concentrate from hematite based low-grade iron ore with high iron recovery rate was con-structed. Impurities contained in iron ore include phosphorus and sulfur in ad-dition to silica and alumina. It is necessary to investigate the process of processing low-grade iron ore considering these impurities in the future.
Acknowledgments and gratitude is hereby expressed to leading program of Aki-ta University “New Frontier Leaders for Rare meAki-tal and Resources”, Japan In-ternational Cooperation Agency (JICA), Japan InIn-ternational Cooperation Centre (JICE) and UMCIL Kafue Steel Plant.
 Ravelomanana, F., Yan, L., Mahazomanana, C. and Miarisoa, L. (2014) Modeling Africa’s Demand for Iron and Steel Importation: An International Market Estima-tion Method Perspective. American Journal of Industrial and Business Manage-ment, 4, 799-815.https://doi.org/10.4236/ajibm.2014.412086
 Umadevi, T., Sah, R. and Mahapatra, P.C. (2014) Influence of Sinter Basicity (CaO/SiO2) on Low and High Alumina Iron Ore Sinter Quality. Mineral Processing
and Extractive Metallurgy, Transactions of the Institutions of Mining and Metal-lurgy, 123, 75-85.
 Svoboda, J. (1994) The Effect of Magnetic Field Strength on the Efficiency of Mag-netic Separation. Mineral Engineering, 7, 747-757.
 Rath, S., Dhawan, N.D., Das, B. and Mishira, B.K. (2014) Optimal Recovery of Iron Values from a Low-Grade Iron Ore Using Reduction Roasting and Magnetic Sepa-ration, Separation Science and Technology, 49, 1927-1936.
DOI: 10.4236/jmmce.2018.63027 393 J. Minerals and Materials Characterization and Engineering
of Polydisperse, Mixed Mineral Particle Systems. Minerals Engineering, 7, 769-791.
 Shao, T.J., Veasey, T.J. and Rowson, N.A. (1996) Wet High-Intensity Magnetic Se-paration of Iron Mineral. Magnetic and electrical Separation, 8, 41-51.
 Rachappa, S. and Prakash, Y. (2015) Iron Ore Recovery from Low Grade by Using Advance Methods. Procedia Earth and Planetary Science, 11, 195-197.
 Araujo, A., Viana, P. and Peres, C. (2005) Reagents in Iron Ore Flotation. Minerals Engineering, 18, 219-224.https://doi.org/10.1016/j.mineng.2004.08.023
 Filippov, L.O., Severov, V.V. and Filippova, I.V. (2014) An Overview of the Bene-ficiation of Iron Ores via Reverse Cationic Flotation. International Journal of Min-eral Processing, 127, 62-69.https://doi.org/10.1016/j.minpro.2014.01.002
 Ana, M.V. and Peres, A.E. (2007) The Effect of Amine Type, pH, and Size Range in the Flotation of Quartz. Minerals Engineering, 20, 1008-1013.
 Chen, L., Zeng, J., Guan, C., Zhang, H. and Yang, R. (2015) High Gradient Magnet-ic Separation in a Centrifugal Field. Minerals Engineering, 78, 122-127.
 Svoboda, J. and Ross, E. (1989) Particle Capture in the Matrix of Magnetic Separa-tor. International Journal of Mineral Processing, 27, 75-94.
 Rachappa, S. and Prakash, Y. (2015) Iron Ore Recovery from Low Grade by Using Advance Methods. Procedia Earth and Planetary Science, 11, 195-197.
 Fuerstenau, D.W. (2005) Zeta Potentials in the Flotation of Oxide and Silicate Min-erals. Advances in Colloid and Interface Science, 114-115, 9-26.
 Fouchee, A., Naude, N., Naik, S.K. and Schommarz, K. (2016) Optimization of Flo-tation pH for the Reverse FloFlo-tation of an African Low-Grade BIF Haematite Ore
Journal of the Southern African Institute of Mining and Metallurgy,116.
 Liu, J.S., Laskowski, Y. and Wang, D. (2010) Effect of Dextrins on the Flotation Re-covery of Molybdenite. Journal of Colloid and Interface Science, 346, 303-310.  Filippov, L.O., Filippova, I.V. and Severov, V.V. (2010) The Use of Collectors
Mix-ture in the Reverse Cationic Flotation of Magnetite Ore; The Role of Fe-Bearing Si-licates. Minerals Engineering, 23, 91-98.
 Rao, K., Hanumantha, F. and Eric, A. (1990) Flotation of Mica Minerals and Selec-tivity between Muscovite and Biotite While Using Mixed Anionic/Cationic Collec-tors. Minerals & Metallurgical Processing, 7, 127-132.
 Kou, J., Tao, D. and Xu, G. (2010) A Study of Adsorption of Dodecyl Amine on Quartz Surface Using Quartz Crystal Microbalance with Dissipation. Colloids and Surfaces A: Physicochemical and Engineering Aspects, 368, 75-83.
 Liu, W., Wei, D. and Cui, B. (2011) Collecting Performances of N-Dodecylethylene-Diamine and Its Adsorption Mechanism on Mineral Surface.
DOI: 10.4236/jmmce.2018.63027 394 J. Minerals and Materials Characterization and Engineering https://doi.org/10.1016/S1003-6326(11)60836-4